SUPERSEDED (click for Active standard)
| ||Format||Pages||Price|| |
|6||$52.80||  ADD TO CART|
1.1 This specification covers carbon and alloy steel pipe, electric-fusion-welded with filler metal added, fabricated from pressure-vessel-quality plate of several analyses and strength levels and suitable for high-pressure service at high temperatures. Heat treatment may or may not be required to attain the desired mechanical properties or to comply with applicable code requirements. Supplementary requirements are provided for use when additional testing or examination is desired.
1.2 The specification nominally covers pipe 16 in. (405 mm) in outside diameter and larger with wall thicknesses up to 3 in. (75 mm) inclusive. Pipe having other dimensions may be furnished provided it complies with all other requirements of this specification.
1.3 Several grades and classes of pipe are provided.
1.3.1 Grade designates the type of plate used as listed in Table 1.
1.3.2 Class designates the type of heat treatment performed in the manufacture of the pipe, whether the weld is radiographically examined, and whether the pipe has been pressure tested as listed in 1.3.3.
1.3.3 Class designations are as follows (Note):Radiography, Pressure Test, Class Heat Treatment on Pipe see Section see Section 10 none none none 11 none 9 none 12 none 9 8.3 13 none none 8.3 20 stress relieved, see 6.3.1 none none 21 stress relieved, see 6.3.1 9 none 22 stress relieved, see 6.3.1 9 8.3 23 stress relieved, see 6.3.1 none 8.3 30 normalized, see 6.3.2 none none 31 normalized, see 6.3.2 9 none 32 normalized, see 6.3.2 9 8.3 33 normalized, see 6.3.2 none 8.3 40 normalized and tempered, see 6.3.3 none none 41 normalized and tempered, see 6.3.3 9 none 42 normalized and tempered, see 6.3.3 9 8.3 43 normalized and tempered, see 6.3.3 none 8.3 50 quenched and tempered, see 6.3.4 none none 51 quenched and tempered, see 6.3.4 9 none 52 quenched and tempered, see 6.3.4 9 8.3 53 quenched and tempered, see 6.3.4 none 8.3
1.4 Optional requirements of a supplementary nature are provided, calling for additional tests and control of repair welding, when desired.
1.5 The values stated in inch-pound units are to be regarded as the standard.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A20/A20M Specification for General Requirements for Steel Plates for Pressure Vessels
A204/A204M Specification for Pressure Vessel Plates, Alloy Steel, Molybdenum
A299/A299M Specification for Pressure Vessel Plates, Carbon Steel, Manganese-Silicon
A370 Test Methods and Definitions for Mechanical Testing of Steel Products
A387/A387M Specification for Pressure Vessel Plates, Alloy Steel, Chromium-Molybdenum
A435/A435M Specification for Straight-Beam Ultrasonic Examination of Steel Plates
A530/A530M Specification for General Requirements for Specialized Carbon and Alloy Steel Pipe
A537/A537M Specification for Pressure Vessel Plates, Heat-Treated, Carbon-Manganese-Silicon Steel
E165 Practice for Liquid Penetrant Examination for General Industry
E709 Guide for Magnetic Particle Testing
ASME Boiler and Pressure Vessel CodeSection IX, Welding Qualifications
UNSPSC Code 40171601(Industrial welded carbon steel pipe)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM A691-98, Standard Specification for Carbon and Alloy Steel Pipe, Electric-Fusion-Welded for High-Pressure Service at High Temperatures, ASTM International, West Conshohocken, PA, 1998, www.astm.orgBack to Top